# diffusion in polymer solids and solutions ... diffusion in polymer solids and solutions 21 .p ds (9)

Post on 03-Mar-2020

0 views

Embed Size (px)

TRANSCRIPT

2

Diffusion in Polymer Solids and Solutions

Mohammad Karimi Amirkabir University of Technology, Department of Textile Chemistry

Iran

1. Introduction

The industrial importance of penetrable and/or impenetrable polymer systems is evident when one faces with a huge number of publications considering various aspects of diffusion phenomenon. Strong worldwide interest to realize more details about the fundamental of the process, generalize the governed laws to new findings, and find fast and reliable techniques of measurement, makes motivation to follow in this field of science. Polymers are penetrable, whilst ceramics, metals, and glasses are generally impenetrable. Diffusion of small molecules through the polymers has significant importance in different scientific and engineering fields such as medicine, textile industry, membrane separations, packaging in food industry, extraction of solvents and of contaminants, and etc. Mass transfer through the polymeric membranes including dense and porous membranes depends on the factors included solubility and diffusivity of the penetrant into the polymer, morphology, fillers, and plasticization. For instance, polymers with high crystallinity usually are less penetrable because the crystallites ordered has fewer holes through which gases may pass (Hedenqvist and Gedde, 1996, Sperling, 2006). Such a story can be applied for impenetrable fillers. In the case of nanocomposites, the penetrants cannot diffuse through the structure directly; they are restricted to take a detour (Neway, 2001, Sridhar, 2006). In the present chapter the author has goals of updating the theory and methodology of diffusion process on recent advances in the field and of providing a framework from which the aspects of this process can be more clarified. It is the intent that this chapter be useful to scientific and industrial activities.

2. Diffusion process

An enormous number of scientific attempts related to various applications of diffusion equation are presented for describing the transport of penetrant molecules through the polymeric membranes or kinetic of sorption/desorption of penetrant in/from the polymer bulk. The mass transfer in the former systems, after a short time, goes to be steady-state, and in the later systems, in all the time, is doing under unsteady-state situation. The first and the second Fick’s laws are the basic formula to model both kinds of systems, respectively (Crank and Park, 1975).

2.1 Fick’s laws of diffusion Diffusion is the process by which penetrant is moved from one part of the system to another

as results of random molecular motion. The fundamental concepts of the mass transfer are

www.intechopen.com

Mass Transfer in Chemical Engineering Processes

18

comparable with those of heat conduction which was adapted for the first time by Fick to

cover quantitative diffusion in an isotropic medium (Crank and Park, 1975). His first law

governs the steady-state diffusion circumstance and without convection, as given by

Equation 1.

c

J D x

(1)

where J is the flux which gives the quantity of penetrant diffusing across unit area of

medium per unit time and has units of mol.cm-2.s-1, D the diffusion coefficient, c the

concentration, x the distance, and /c x is called the gradiant of the concentration along the axis. If J and c are both expressed in terms of the same unit of quantity, e.g. gram, then

D is independent of the unit and has unit of cm2.s-1. Equation 1 is the starting point of

numerous models of diffusion in polymer systems. Simple schematic representation of the

concentration profile of the penetrant during the diffusion process between two boundaries

is shown in Fig. 1-a. The first law can only be directly applied to diffusion in the steady

state, whereas concentration is not varying with time (Comyn, 1985). Under unsteady state circumstance at which the penetrant accumulates in the certain

element of the system, Fick’s second law describes the diffusion process as given by

Equation 2 (Comyn, 1985, Crank and Park, 1968).

c c D

t x x

(2) Equation 2 stands for concentration change of penetrant at certain element of the system

with respect to the time ( t ), for one-dimensional diffusion, say in the x-direction.

Diffusion coefficient, D , is available after an appropriate mathematical treatment of kinetic

data. A well-known solution was developed by Crank at which it is more suitable to

moderate and long time approximation (Crank, 1975). Sorption kinetics is one of the most

common experimental techniques to study the diffusion of small molecules in polymers. In

this technique, a polymer film of thickness 2l is immersed into the infinit bath of penetrant, then concentrations, tc , at any spot within the film at time t is given by Equation 3

(Comyn, 1985).

2 2

2 0

4 1 2 1 2 1 1

2 1 24

( ) ( ) ( ) exp cos

n t

n

c D n t n x

c n ll

(3) where c is the amount of accumulated penetrant at equilibrium, i.e. the saturation equilibrium concentration within the system. 2L l is the distance between two boundaries layers, x0 and x1 (Fig. 1-b).

Integrating Equation 3 yields Equation 4 giving the mass of sorbed penetrant by the film as

a function of time t , tM , and compared with the equilibrium mass, M .

2 2

2 2 2 0

8 2 1 1

2 1 4

( ) exp

( ) t

n

M D n t

M n l

(4)

www.intechopen.com

Diffusion in Polymer Solids and Solutions

19

Fig. 1. Concentration profile under (a) steady state and (b) unsteady state condition.

For the processes which takes place at short times, Equation 4 can be written, for a thickness

of 2L l , as

1 2

1 2

2tM D t M l

(5) Plotting the /tM M as function of

1 2t , diffusion coefficient can be determine from the

linear portion of the curve, as shown in Fig. 2. Using Equation 5 instead of Equation 4, the

error is in the range of 0.1% when the ratio of /tM M is lower than 0.5 (Vergnaud, 1991).

In the case of long-time diffusion by which there may be limited data at 0 5/ .tM M , Equation 4 can be written as follow:

2

2 2

8 1

4 expt

M D t

M l

(6) Equation 6 is usually used in the form of Equation 7, as given following,

2

2 2

8 1

4 ln lnt

M D t

M l

(7) This estimation also shows similarly negligible error on the order of 0.1% (Vergnaud, 1991).

Beyond the diffusion coefficient, the thickness of the film is so much important parameter

affected the kinetics of diffusion, as seen in Equation 4. The process of dyeing by which the

dye molecules accumulate in the fiber under a non-linear concentration gradient is known

as the unsteady-state mass transfer, since the amount of dye in the fiber is continuously

increasing. Following, Equation 8, was developed by Hill for describing the diffusion of dye

molecules into an infinitely long cylinder or filament of radius r (Crank and Park, 1975,

Jones, 1989).

www.intechopen.com

Mass Transfer in Chemical Engineering Processes

20

0 2 4 6 8 10 12 0.0

0.2

0.4

0.6

0.8

1.0

1.2

a

D=1.0*10-10 cm2/sec 2l=15 m

M t/M

in f

t1/2 0 5 10 15 20 25 30 35

-1.0

-0.8

-0.6

-0.4

-0.2

0.0

D=1.0*10-10 cm2/sec 2l=15 m

ln (1

-M t/M

in f)

t (min)

b

Fig. 2. Kinetics of mass uptake for a typical polymer. (a) /tM M as function of 1

2t , (b)

1ln( / )tM M as function of t ; data were extracted from literature (Fieldson and Barbari, 1993).

2 2

2 2

2

1 0 692 5 785 0 190 30 5

0 0775 74 9 0 0415 139

0 0258 223

. exp . / . exp . /

. exp . / . exp /

. exp / ....)

tC Dt r Dt r C

Dt r Dt r

Dt r

(8)

Variation of /tC C for different values of radius of filaments are presented in Fig. 3. As seen in Fig.3, decreasing in radius of filament causes increasing in the rate of saturating.

0 200 400 600 800 1000 0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

1.0

1.1

c t /c

in f

time (sec)

Radius of filament = 30 m Radius of filament = 20 m Radius of filament = 14 m Radius of filament = 9 m

Fig. 3. /tC C of dyeing versus t for different radius of